| ||Format||Pages||Price|| |
|9||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$48.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$58.00||  ADD TO CART|
Significance and Use
4.1 The myriad array of particle size analysis techniques available to the modern-day powder technologist is both daunting and confusing. Many of the techniques are applicable only to certain types of materials, and all have limited ranges of applicability with respect to powder particle size. This guide is an attempt to describe and define the applicability of each of the available techniques, so that powder technologists, and others interested in powders, may make informed and appropriate choices in characterizing their materials.
4.2 This guide is intended to be used to determine the best and most efficient way of characterizing the particle size distribution of a particular powder material. It may also be used to determine whether a reported powder particle size, or size distribution, was obtained in an appropriate and meaningful way.
4.3 Most particle size analysis techniques report particle size in terms of an “equivalent spherical diameter”: the diameter of an ideal spherical particle of the material of interest that would be detected in the same manner during analysis as the (usually irregular-shaped) actual particle under the same conditions. The different techniques must necessarily use different definitions of the equivalent spherical diameter, based on their different operating principles. However, when analyzing elongated particles, the size parameter most relevant to the intended application should be measured; for example, length (maximum dimension).
4.4 Reported particle size measurement is a function of both the actual dimension or shape factor, or both, as well as the particular physical or chemical properties of the particle being measured. Caution is required when comparing data from instruments operating on different physical or chemical parameters or with different particle size measurement ranges. Sample acquisition, handling, and preparation can also affect reported particle size results.
1.1 This guide covers the use of many available techniques for particle size measurement and particle size distribution analysis of solid particulate (powder) materials, off-line in a laboratory. It does not apply to in-line (on-line) analysis, nor to analysis of liquid droplets or liquid aerosols. The guide is intended to serve as a resource for powder/particle technologists in characterizing their materials.
1.2 This guide provides significant detail regarding the numerous particle size analysis methods available. Although this guide is extensive, it may not be all inclusive.
1.3 The principle of operation, range of applicability, specific requirements (if any), and limitations of each of the included particle size analysis techniques are listed and described, so that users of this guide may choose the most useful and most efficient technique for characterizing the particle size distribution of their particular material(s).
1.4 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.6 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B215 Practices for Sampling Metal Powders
B330 Test Methods for Estimating Average Particle Size of Metal Powders and Related Compounds Using Air Permeability
B821 Guide for Liquid Dispersion of Metal Powders and Related Compounds for Particle Size Analysis
B859 Practice for De-Agglomeration of Refractory Metal Powders and Their Compounds Prior to Particle Size Analysis
C322 Practice for Sampling Ceramic Whiteware Clays
E11 Specification for Woven Wire Test Sieve Cloth and Test Sieves
E161 Specification for Electroformed Material and Test Sieves
E1617 Practice for Reporting Particle Size Characterization Data
E1638 Terminology Relating to Sieves, Sieving Methods, and Screening Media
E2589 Terminology Relating to Nonsieving Methods of Powder Characterization
ICS Number Code 19.120 (Particle size analysis. Sieving)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E2651-19, Standard Guide for Powder Particle Size Analysis, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top